- Failure theory (material)
Materials failure modes Continuum mechanics
Failure theory is the science of predicting the conditions under which solid materials fail under the action of external loads. The failure of a material is usually classified into brittle failure (fracture) or ductile failure (yield). Depending on the conditions (such as temperature, state of stress, loading rate) most materials can fail in a brittle or ductile manner or both. However, for most practical situations, a material may be classified as either brittle or ductile. Though failure theory has been in development for over 200 years, its level of acceptability is yet to reach that of continuum mechanics.
In mathematical terms, failure theory is expressed in the form of various failure criteria which are valid for specific materials. Failure criteria are functions in stress or strain space which separate "failed" states from "unfailed" states. A precise physical definition of a "failed" state is not easily quantified and several working definitions are in use in the engineering community. Quite often, phenomenological failure criteria of the same form are used to predict brittle failure and ductile yield.
- 1 Material failure
- 2 Types of material failure
- 3 Brittle material failure criteria
- 4 Ductile material failure criteria
- 5 See also
- 6 References
- 7 External links
In materials science, material failure is the loss of load carrying capacity of a material unit. This definition per se introduces the fact that material failure can be examined in different scales, from microscopic, to macroscopic. In structural problems, where the structural response may be beyond the initiation of nonlinear material behaviour, material failure is of profound importance for the determination of the integrity of the structure. On the other hand, due to the lack of globally accepted fracture criteria, the determination of the structure's damage, due to material failure, is still under intensive research.
Types of material failure
Material failure can be distinguished in two broader categories depending on the scale in which the material is examined:
Microscopic material failure is defined in terms of crack propagation and initiation. Such methodologies are useful for gaining insight in the cracking of specimens and simple structures under well defined global load distributions. Microscopic failure considers the initiation and propagation of a crack. Failure criteria in this case are bhanu related to microscopic fracture. Some of the most popular failure models in this area are the micromechanical failure models, which combine the advantages of continuum mechanics and classical fracture mechanics. Such models are based on the concept that during plastic deformation, microvoids nucleate and grow until a local plastic neck or fracture of the intervoid matrix occurs, which causes the coalescence of neighbouring voids. Such a model, proposed by Gurson and extended by Tvergaard and Needleman, is known as GTN. Another approach, proposed by Rousselier, is based on continuum damage mechanics (CDM) and thermodynamics. Both models form a modification of the von Mises yield potential by introducing a scalar damage quantity, which represents the void volume fraction of cavities, the porosity f.
Macroscopic material failure is defined in terms of load carrying capacity or energy storage capacity, equivalently. Li presents a classification of macroscopic failure criteria in four categories:
- Stress or strain failure
- Energy type failure (S-criterion, T-criterion)
- Damage failure
- Empirical failure.
Five general levels are considered, at which the meaning of deformation and failure is interpreted differently: the structural element scale, the macroscopic scale where macroscopic stress and strain are defined, the mesoscale which is represented by a typical void, the microscale and the atomic scale. The material behaviour at one level is considered as a collective of its behaviour at a sublevel. An efficient deformation and failure model should be consistent at every level.
Brittle material failure criteria
Failure of brittle materials can be determined using several approaches:
- Phenomenological failure criteria
- Linear elastic fracture mechanics
- elastic-plastic fracture mechanics
- Energy-based methods
- Cohesive zone methods
Phenomenological failure criteria
The failure criteria that were developed for brittle solids were the maximum stress/strain criteria. The maximum stress criterion assumes that a material fails when the maximum principal stress σ1 in a material element exceeds the uniaxial tensile strength of the material. Alternatively, the material will fail if the minimum principal stress σ3 is less than the uniaxial compressive strength of the material. If the uniaxial tensile strength of the material is σt and the uniaxial compressive strength is σc, then the safe region for the material is assumed to be
Note that the convention that tension is positive has been used in the above expression.
The maximum strain criterion has a similar form except that the principal strains are compared with experimentall determined uniaxial strains at failure, i.e.,
The maximum principal stress and strain criteria continue to be widely used in spite of severe shortcomings.
Numerous other phenomenological failure criteria can be found in the engineering literature. The degree of success of these criteria in predicting failure has been limited. For brittle materials, some popular failure criteria are
- criteria based on invariants of the Cauchy stress tensor
- the Tresca or maximum shear stress failure criterion
- the von Mises or maximum elastic distortional energy criterion
- the Mohr-Coulomb failure criterion for cohesive-frictional solids
- the Drucker-Prager failure criterion for pressure-dependent solids
- the Bresler-Pister failure criterion for concrete
- the Willam-Warnke failure criterion for concrete
- the Hankinson criterion, an empirical failure criterion that is used for orthotropic materials such as wood.
- the Hill yield criteria for anisotropic solids
- the Tsai-Wu failure criterion for anisotropic composites
- the Johnson–Holmquist damage model for high-rate deformations of isotropic solids
- the Hoek-Brown failure criterion for rock masses
Linear elastic fracture mechanics
The approach taken in linear elastic fracture mechanics is to estimate the amount of energy needed to grow a preexisting crack in a brittle material. The earliest fracture mechanics approach for unstable crack growth is Griffiths' theory . When applied to the mode I opening of a crack, Griffiths' theory predicts that the critical stress (σ) needed to propagate the crack is given by
where E is the Young's modulus of the material, γ is the surface energy per unit area of the crack, and a is the crack length for edge cracks or 2a is the crack length for plane cracks. The quantity is postulated as a material parameter called the fracture toughness. The mode I fracture toughness for plane strain is defined as
where σc is a critical value of the far field stress and Y is a dimensionless factor that depends on the geometry, material properties, and loading condition. The quantity KIc is related to the stress intensity factor and is determined experimentally. Similar quantities KIIc and KIIIc can be determined for mode II and model III loading conditions.
The state of stress around cracks of various shapes can be expressed in terms of their stress intensity factors. Linear elastic fracture mechanics predicts that a crack will extend when the stress intensity factor at the crack tip is greater than the fracture toughness of the material. Therefore the critical applied stress can also be determined once the stress intensity factor at a crack tip is known.
The linear elastic fracture mechanics method is difficult to apply for anisotropic materials (such as composites) or for situations where the loading or the geometry are complex. The strain energy release rate approach has proved quite useful for such situations. The strain energy release rate for a mode I crack which runs through the thickness of a plate is defined as
where P is the applied load, t is the thickness of the plate, u is the displacement at the point of application of the load due to crack growth, and a is the crack length for edge cracks or 2a is the crack length for plane cracks. The crack is expected to propagate when the strain energy release rate exceeds a critical value GIc - called the critical strain energy release rate.
The fracture toughness and the critical strain energy release rate for plane stress are related by
where E is the Young's modulus. If an initial crack size is known, then a critical stress can be determined using the strain energy release rate criterion.
Ductile material failure criteria
Criteria used to predict the failure of ductile materials are usually called yield criteria. Commonly used failure criteria for ductile materials are:
- the Tresca or maximum shear stress criterion.
- the von Mises yield criterion or distortional strain energy density criterion.
- the Gurson yield criterion for pressure-dependent metals.
- the Hosford yield criterion for metals.
- the Hill yield criteria.
- various criteria based on the invariants of the Cauchy stress tensor.
The yield surface of a ductile material usually changes as the material experiences increased deformation. Models for the evolution of the yield surface with increasing strain, temperature, and strain rate are used in conjunction with the above failure criteria for isotropic hardening, kinematic hardening, and viscoplasticity. Some such models are:
- the Johnson-Cook model
- the Steinberg-Guinan model
- the Zerilli-Armstrong model
- the Mechanical threshold stress model
- the Preston-Tonks-Wallace model
There is another important aspect to ductile materials - the prediction of the ultimate failure strength of a ductile material. Several models for predicting the ultimate strength have been used by the engineering community with varying levels of success. For metals, such failure criteria are usually expressed in terms of a combination of porosity and strain to failure or in terms of a damage parameter.
- Fracture mechanics
- Stress intensity factor
- Yield (engineering)
- Yield surface
- Plasticity (physics)
- Structural failure
- Strength of materials
- Ultimate failure
- ^ Besson J., Steglich D., Brocks W. (2003), Modelling of plain strain ductile rupture, International Journal of Plasticity, 19.
- ^ Li, Q.M. (2001), Strain energy density failure criterion, International Journal of Solids and Structures 38, pp. 6997–7013.
- ^ Griffiths,A.A. 1920. The theory of rupture and flow in solids. Phil.Trans.Roy.Soc.Lond. A221, 163.
Wikimedia Foundation. 2010.
Look at other dictionaries:
Theory of constraints — Part of a series of articles on Industry Manufacturing methods Batch production • Job production Continuous production Improvement method … Wikipedia
theory — A reasoned explanation of known facts or phenomena that serves as a basis of investigation by which to seek the truth. SEE ALSO: hypothesis, postulate. [G. theoria, a beholding, speculation, t., fr. theoros, a beholder] adsorption t. of narcosis… … Medical dictionary
Christensen Failure Criterion — Failure criteria for isotropic materials has been a long standing problem. Despite many historical attempts, there have not been any successful general forms that span the range from ductile to brittle materials. A new failure criterion that aims … Wikipedia
Micro-Mechanics of Failure — Figure 1. Hierarchy of micromechanics based analysis procedure for composite structures. Micro Mechanics of Failure (MMF) is a newly proposed methodology, providing a more logical explanation of failure mechanism of continuous f … Wikipedia
Tsai-Wu failure criterion — The Tsai Wu failure criterion [Tsai, S. W. and Wu, E. M. (1971). A general theory of strength for anisotropic materials. Journal of Composite Materials. vol. 5, pp. 58 80.] is a phenomenological failure theory which is widely used for anisotropic … Wikipedia
Mohr–Coulomb theory — Continuum mechanics … Wikipedia
Finite strain theory — Continuum mechanics … Wikipedia
Strain theory (sociology) — In criminology, the strain theory states that social structures within society may encourage citizens to commit crime. Following on the work of Émile Durkheim, Strain Theories have been advanced by Merton (1938), Cohen (1955), Cloward and Ohlin… … Wikipedia
Mohr-Coulomb theory — is a mathematical model (see yield surface) describing the response of a material such as rubble piles or concrete to shear stress as well as normal stress. Most of the classical engineering materials somehow follow this rule in at least a… … Wikipedia
Jesus myth theory — The Resurrection of Christ by Noel Coypel (1700). Jesus myth theorists see this as one of a number of stories about dying and rising gods. Description The … Wikipedia